FORGING BLADES SINCE THE IRON AGE
Steels are a class of materials with multiple and complicated transformations; this is true even for steels of the basic cutlery industry. A damascus steel is a fascinating subject to study, rich in multiple facets, that appears in a ﬁ rst approach as a composite material artistically exploited.
Damacus steel was developed in the ﬁ rst millennium AD in India or Sri-Lanka. Its reputation is related to its exceptional properties and to the moire pattern. A similar damask pattern could be obtained by forge-welding giving rise to controversies. Recent ﬁ ndings allow a better understanding of this pattern formation.
This book presents ﬁ rstly, observations of ancient blade samples examined with modern technologies such as electron microscopy. The features of many typical swords from different periods are discussed:
Celtic, Merovingian, Viking and oriental wootz swords, Persian shamshirs, Japanese katana, rapiers etc. In the second part, microstructural observations at different levels of magniﬁ cation are displayed and their interpretation is discussed in detail, thus revealing the secret of sophisticated forgings. One chapter is devoted to introducing the main transformations undergone by these steels during the forging processes.
The book is intended for all those people interested in the history of science and more speciﬁ cally to the metallurgists, to the archaeologists and all the researchers confronted with the problems of the expertise of the vestiges, to the blacksmiths, and to the collectors of valuable artistic blades.
Madeleine Durand-Charre has taught structural metallurgy at the Polytechnic Institute of Grenoble and at the University Joseph Fourier of Grenoble. Her research work concerned microstructure formation and determination of phase equilibria. She investigated complex alloys such as superalloys and steels. Her work on vanadium cast irons was awarded the Vanadium Shield in 1989 from the Institute of Metals. She is author of several books and articles in metallurgy.
ISBN : 978-2-7598-1173-1 / 49 € www.edpsciences.org
DAMASCUS AND PATTERN-WELDED STEELS MAdeleine Dur
metallurgy I materials
materials I metallurgy
Forging blades since the iron age
This new book is an updated translation from French of “Les aciers damassés. Du fer primitif aux aciers modernes” (Presses des Mines, 2007).
Books by the same author:
“The microstructure of superalloys” (Gordon and Breach, 1997)
“La microstructure des aciers et des fontes” (SIRPE, 2003 and EDP, 2012)
“Microstructure of steels and cast irons” (Springer, 2004, translated from French version here above)
Printed in France
This work is subject to copyright. All rights are reserved, whether the whole or part of the material is concerned, specifically the rights of translation, reprinting, re-use of illustrations, recitation, broad-casting, reproduction on microfilms or in other ways, and storage in data bank. Duplication of this publication or parts thereof is only permitted under the provisions of the French Copyright law of March 11, 1957. Violations fall under the prosecution act of the French Copyright law.
© EDP Sciences 2014
Table of contents
Introduction . . . III Aknowledgments . . . V
First part :
The Blacksmith’s steel spanning four millennia
1 Primitive iron
1.1 Iron before the Iron Age . . . 3
1.2 Early iron making techniques . . . 7
1.3 The mythical aspects of iron . . . 12
1.4 Archaeological remains . . . 15
2 Blacksmith steel before the Christian era 2.1 The swords/daggers of Loristan . . . 19
2.2 The Celtic sword-making tradition . . . 22
2.3 The Etruscan swords . . . 31
3 The swords of the first millennium AD 3.1 Merovingian (481-751) and Carolingian (after 751) swords . . . 33
3.2 The Vikings swords . . . 40
3.3 Swords in China . . . 45
3.4 Swords forged with crucible steel . . . 45
4 Did you say Damascus steel, Damascene or damask ? 4.1 The debate on the origin of the naming . . . 47
4.2 From laminated to figurative blades . . . 48
4.3 Crystallization steel or pattern-welded steel . . . 51
4.4 Damaskeen, damaskeened, damascene . . . 53
5 From swords to knives 5.1 The lake of Paladru . . . 55
5.2 The knives at the beginning of the millennium, in the year one thousand . . . . 57
6 The swords of the second millennium 6.1 The use of the sword in Europe . . . 63
6.2 Damask rapiers . . . 65
6.3 The engraved steel imitates and competes with the damasked steel . . . 68
6.4 Making gun barrels with damask . . . 69
6.5 The pattern-welded oriental swords . . . 73
6.6 Swords made with Damascus steel . . . 78
6.7 Japanese swords . . . 83
7 Art and Technology in the third millennium 7.1 The Renaissance of an art and craft . . . 91
7.2 The search for the best cutting edge . . . 92
7.3 Multilayer steels . . . 98
7.4 Inserts and mosaic patterns . . . 105
7.5 Sintered steels . . . 110
7.6 The colored blades . . . 115
7.7 The contemporary wootz . . . 119
Second part : Formation of the damask pattern8 Understanding steels 8.1 Phases and phase diagrams . . . 127
8.2 Austenite transformation in the Fe-C system . . . 132
8.3 Kinetics of the austenite transformation . . . 136
8.4 Heat treatments . . . 140
8.5 Solidification structure . . . 143
8.6 Dendritic segregation . . . 145
8.7 Steels used for cutlery . . . 148
8.8 Optimizing microstructure . . . 151
8.9 Coloration of stainless steels . . . 154
8.10 Powder metallurgy . . . 156
9 Pattern-welding 9.1 Welding different layers . . . 159
10 Moire pattern in wootz type, high carbon steels 10.1 Crucible steels (wootz, pulad) . . . 169
10.2 Formation of the moire pattern . . . 170
10.3 Structure of the matrix . . . 180
11 Alignments in medium carbon steels 11.1 A well-known phenomenon . . . 189
11.2 Occurrence of banding in ancient steels . . . 193
11.3 The contribution of structural metallurgy . . . 199
12 References List of references . . . 203
13 Index Index . . . 211
Trying to understand what a damask steel is, I discovered a fascinating subject, rich in multiple facets which initially appears simple: this is laminated steel, a composite material artistically exploited. In fact, the name is confusing when considering the words refering to Damascus such as damask, damascene and Damascus steels have different meanings and refer to very different materials whose common feature is just a wavy pattern.
During the first millennium BC the Celtic smiths acquired control of hot iron working, in particular for the production of strong sword blades. The latter were built by forge welding more or less carburized pieces of smelted iron. Damask steel appears as a pattern-welded composite resulting from this know-how several centu- ries later.
Meanwhile, in Eastern countries a high carbon steel was developped. This legen- dary steel displayed a moire pattern after specific forging. It was known by several names, Indian steel, Damascus steel or wootz etc. and remained rather mysterious until the 17th century. The history of the debate comparing the different kinds of steels is evoked in chapter 4.
Since this period, modern sophisticated tools became available to observe the speci- mens. Many researchers, in particular the Verhoeven team, investigated the micros- tructure of ancient blades, thus enabling clarification of how they were forged. This is the point of view that I plan to develop in detail.
What readers are likely to be interested by this subject?
- Metallurgists, I thought about my colleagues because I regretted, after having taught the structural metallurgy during many years, not having opened a very small window, a few minutes in my timetable to explain to the students how the metal- lurgy of iron has developed.
- Archaeologists, the curators of a museum and all the researchers confronted with the problems of expertises of the vestiges. They can, therefore, be interested by a detailed approach to the micrographic aspects.
- Blacksmiths who have a good technical approach to metallurgy supported by sound experimental know-how. They participate on the Internet in numerous discus- sion forums. As an occasional observer, I noted some points for which a funda- mental approach could be useful.
- Collectors and amateurs who appreciate to be informed of the making of their valuable artistic blades.
However, when writing this book it appeared difficult to me to address such diffe- rent readers, to avoid specialist's vocabulary and find a common language. That is why the text has been divided into two parts. A first descriptive part which presents the developments in the technology of forging in various places and various periods, and a more fundamental second part with the aim of explaining the scien- tific mechanisms and present the most recent findings for the formation of parti- cular microstructures such as the bands or alignments responsible for the moire structure.
However, steels are a material with multiple and complicated transformations ; this is true even for steels of basic cutlery industry. The explanation of a mechanism requires a detailed description in order to respect a strict argumentation. To ensure a sound basis to the discussion in its scientific context, the concepts of phase, grain, segregation and the particular features of high carbon steels are revisited in chapter 8. This edition is supplemented with a few new examples, with tables summarizing the findings and an index. Ultimately, this book does not propose practical solutions to the blacksmiths but rather a microscopic vision of their metal in order to support a better understanding of the formation of the microstructure.
Madeleine Durand-Charre [email protected]
To acheive this work I ventured a little imprudently out of my strict scientific disci- pline. Also it was necessary for me to ask for the assistance of specialists in other disciplines extremely far away from mine. I express my gratitude to all those who believed in this project and who allowed the use of documents or samples, or prepared specific photographs.
I will quote in particular MM Paul Merluzzo, Louis Bonamour, Eric Perrin and Ernst Kläy. Many archaeologists, researchers, curators of a museum, transmitted documents or information to me : Mmes Christine Bouclet-Riquier, Véronique Despine, Anna Feuerbach, M.C. Lebascle, Aurélie R. v.Bieberstein, Bernadette Schnitzler, C. Vigouroux, et MM Gilles Desplanque, M. Ferry, Leon Kapp, J.
Parisot, Jean Renaud, O. Renaudeau, J. P. Sage, Philippe Schaffnit, Pierre Thomas, Eric Verdel, John Verhoeven and Yoshindo Yoshihara.
My project began with my professional retirement when I had time available but I did not have any more the daily contact with my former laboratory at the Poly- technic Institute of Grenoble (INPG). Micrographs coming from my work of research, almost the memories of a photo album, were not sufficient. I am particu- larly indebted to my former colleagues and friends Annie Antoni, Florence Robault, Catherine Tassin and Muriel Véron for fruitful discussions and their assistance to supplement some examinations, analyses or micrographs.
I thank the blacksmiths, the knifemakers, the engineers and François-Xavier Salle, chief editor of “La passion des couteaux” who enabled me to give an outline of the original achievements of the contemporary artistic crafts : Olivier Bertrand, Per Bilgren, Alain et Joris Chomillier, Des Horn, Sébastien Masson, Matthieu Petitjean, Eric Plazen, François Pitaud, Denis Pittet, Pierre Reverdy, Manfred Sachse, Henri Viallon and Achim Wirtz.
I thank Jean Giraud (Moebius) for the permission to use a drawing, François Chabanne for the access to ancient books, as well as Micheline Mosselmans and Sonia Durand for their contributions to the drawings.
First part :
The Blacksmith’s steel
spanning four millennia
1.1 Iron before the Iron Age
The metallurgy of iron appeared in most ancient societies subsequent to that of gold and that of copper. The most significant appearance was situated in Anatolia in the Hittites, between 1400 and 1700 BC, thus determines the beginning of the Iron Age. The oldest discoveries date back to the prehistoric period around 5000 years BC in Iraq (Samara), in Iran (Tepe Sialk) and in Egypt (El Gerseh). More recently, discove- ries in the period known as the bronze age (3000–1600 BC) are all situated on a wide border East and Southeast of the Mediterranean Basin in Mesopotamia, Turkey, Egypt and Cyprus (more details can be found in ).
Furthermore, the presence of objects made from iron does not necessa- rily imply the ability to extract the metal from its ores, since iron also exists in native and particularly meteoritic forms, although the sources are by no means abundant.
The earliest iron used by man was generally meteoritic in origin. It is the presence of nickel which distinguishes it from the other categories of iron. Modern characterization techniques enabled detecting that nic- kel is present in most objects of the prehistoric period and in those from the early and middle bronze ages. The iron found as metallic meteorites, called also siderites (Figure 1.1.1), were worked in the same way as stone in order to form tools. In Greenland, three meteori- tes among the largest ever found (one weighed 36 tonnes) had been used for generations by Eskimos.
In Central and South America, the Aztecs, Mayas and Incas used meteoritic iron well before knowing its metallurgy. They considered it
Figure 1.1.1 :
Polished section of a metallic meteorite from a multiple fall, known under the name of Gibbeon (Namibia). To notice the Widmanstätten structure consisting in long needles imbricated along three directions.
Courtesy ENS Lyon, Fr.
Meteoritic iron is an alloy which generally contains a few percent of nickel, with amounts ranging from 5 to 26%, together with small amounts of cobalt (up to 1%) and traces of sulfur, phosphorus and car- bon. Metallic meteorites are relatively malleable. They are one of the three major classes of meteorites, corresponding to metallic, stoney and mixed structures . They are generally believed to be fragments of planets that have disintegrated, the metallic meteorites emanating from deep inner layers. The crystalline phases present in metallic meteorites have names specific to this field of study. For low nickel concentrations, the body-centered cubic crystal structure is known as kamacite (α ferrite in steels, §8.1), whereas the face-centered cubic structure found in high nickel meteorites is called tænite (γ austenite in steels). This structure consists of plate-like ferrite and was observed for the first time in 1808 in a meteorite by Aloïs von Beckh Widmans- tätten (Figure 1.1.1). The plates are oriented in directions which form an octahedron. The origin of this structure in meteorites has been sug- gested to be associated with the existence of a solid state reaction at very high pressures . However, for certain meteorites the micros- tructure is so coarse, with broad plates several millimeters, that a solid state transformation could seems unlikely .
Telluric iron may be found in the native state in basalt or other rocks as small grains or nodules. It often contains a high content of nickel, up to 70%. This iron, rarer than the meteoritic iron, was sometimes found in precious objects. Ural native iron contains 50 % of platinum.
The name terrestrial iron is given to iron extracted from ores ; it is nor- mally free from nickel. Iron of this type has been found in objects in Egypt, in the Temple valley and Cheops' pyramid at Giza (2500 BC) and at Abydos (2200 BC). However, the number of such objects is small and their authenticity is doubtful, due to their poor state of con- servation.
The oldest iron not of meteoritic or native origin is found as small decorative inlays in gold jewellery or tiny cult objects. It has been sug- gested that this iron is a by-product of the gold production process.
Magnetite is frequently present in the gold-bearing sands in Nubia and could have been reduced during the smelting operation as pasty iron floating in the slag above the molten gold. Another possibility is that iron oxides were deliberately associated with other oxides used as fluxes for the manufacture of bronze. The iron dating from this period was described as accidental iron .
Whether the production of iron by the reduction of ores was discovered at an early stage, before 2000 BC is a subject of controversy. All the more, the presence of non-meteoritic iron objects is not always asso- ciated with evidence of local mining activities. For example, in Egypt, where iron ore deposits are abundant, there is no sign of their exploita- tion. The argument is that it is probably due to the absence of forests capable of supplying the charcoal necessary for reduction.
Recent investigations with modern means of analysis have evidenced that a bead from the prehistoric Gerzeh cemetery, approximately 3300 BC, which was considered as the earliest example of exploitation of iron in Egypt, was in fact made out of cold-worked meteoritic iron .
It must be remarked that several millennia elapsed between the first reliable identifications of iron artifacts and the start of what can be genuinely termed the iron age. Several explanations can be suggested.
The most obvious one is the inherent difficulty of extracting iron from its ores. The processes used for gold and copper are not applicable, and in particular, much higher temperatures are required.
It is difficult to forget what we know about iron to imagine how this new material was considered. In fact, the iron obtained by the most pri- mitive processes of reduction of the ore should not have been regarded as an interesting material. When iron is reduced, it is pure and highly malleable, thus usable only for ornaments. It was rare, and therefore very precious and its value could exceed several tens of times that of gold.
After aluminum, iron is the second most abundant metal in the Earth's crust. The major iron ores are essentially oxides (magnetite Fe2O3, hematite Fe3O4 and limonite), carbonates (siderite) and sulphides (pyrite). The preparation by washing and crushing of the ore is the same one as that practiced for the other ores. Many ore deposits occur in the eastern Mediterranean basin and can often be readily recognized due to the associated rust-red coloration of the earth. Indeed, they were often exploited as pigments, giving the yellows, ochres, browns and reds used by the Egyptians. Evidence of early mining activities is visi- ble in deposits in Syria and Cappadocia, which appear to have been the first to be exploited on a large scale. Metallurgical culture is extremely ancient throughout the fertile crescent, facilitated by the presence of numerous rich ore deposits. The Assyrians seem to have practiced the reduction of iron ore as early as the 19th century BC.
Some ores were famous, probably due to the natural presence of alloying elements such as manganese (Siegerland in Germany), nickel (Greek or Corsican ores) or phosphorus (Lorraine ore) [7-8].
In the earliest iron processes, washed and crushed ore was heated with charcoal in a primitive furnace, often consisting of little more than a hole in the ground. The temperature attained was insufficient to achieve melting and the oxide was reduced by the carbon in the solid state, leading to a spongy agglomerate called a bloom. Many primitive furnaces were built in such a way as to optimize natural drought (Sri Lanka). Furthermore, the use of rudimentary bellows made from ani- mal hide was probably adopted at an early stage. The furnace can be controlled by the injection of air and, depending on the setting, local carburization of the iron can be acheived. This carburization occurs at high temperature by contact of the iron with a CO atmosphere near the charcoal. Traces of cast iron found amongst the slag in ancient smelting centers indicates that the temperatures attained were suffi- ciently high to induce partial melting. However, such cast iron was probably initially obtained accidentally and considered as a worthless by-product, since it was hard, brittle and unworkable.
The development of iron smelting was particularly facilitated in areas where ore deposits were associated with ready supplies of charcoal and refractory materials for furnace construction.
The smelting stage produces a spongy agglomerate called a bloom, consisting of well reduced iron particles, residual oxide inclusions and areas with carburized iron particles. The bloom has to be repeatedly heated and hammered to expel residual slag inclusions, forming a more compact mass. The addition of sand during reheating contributes to the removal of oxide inclusions by the formation of a fusible envelope of fayalite. The iron obtained in this way was fairly pure, since oxides of other metallic elements such as Si or Al could not be reduced in these conditions. Its carbon content is low, it is therefore malleable.
Pure iron can be carburized by simple welding in contact with more carburized iron agglomerates during repeated hot hammering. If the metal working is intense, the agglomerates are crushed, mixed and car- bon diffuses between the iron grains, it results in a homogenization of its concentration.
The soft iron can also be carburized by a further treatment known as cementation whereby carbon difffuses into the metal. At the temperatu- res attained, the depth of carbon penetration was no more than about a millimeter (see Table 8.1.2). Thus, this process can be carried out only locally to strengthen superficial areas, or sharp edges, or on iron divi- ded into pellets or thin strips. Prakash underlines that the Indian blacksmiths had acquired a great knowledge of the effects of carbon in iron and knew how to control the production of more or less carburized iron .
Crucible steel in East Asia
The fusion of steel in a crucible is an invention of the first millennium BC. The production of crucible steel goes back to 300 BC according to the history of the wootz written by Srinivasan and Ranganathan at the University of Bangalore in India, [10-11]. This date is based on the dis- covery of high-carbon steel on a production site of this period (Kodu- manal). This vestige is the oldest known, it is presented as a relatively reliable proof of the more or less complete fusion of the steel.
The same authors also quote a document according to which, Indian king Pôros, defeated by Alexander Great, offered to his conqueror 30
Recent excavations revealed several sites of production in Central Asia, among them Merv in Turkmenistan and Achsiket in Uzbekistan.
The oasis of Merv located on the silk route was an important produc- tion center in the 8th et 9th centuries. Anna Feuerbach, who took part in excavations, presents in several publications an example of exploita- tion of vestiges led in a rigorous scientific way [12-15]. The sites of Achsiket are dated between the 9th and 14th centuries.
The iron as reduced from its ore was melted in a crucible in a distinct subsequent operation. Steel was prepared by small charges, each con- sisting mainly of iron, charcoal of bamboo and leaves of specific plants. The iron used was probably in the form of an iron sponge, it still contained oxides particles which while melting form a protective slag at the surface of the ingot. The whole was then hermetically sealed in clay crucibles. A batch of some twenty crucibles was heated for a long time at temperatures up to 1200°C, and then let cool. Liquid iron was carburized by reaction with charcoal enabling a partial melting [12-13].
The iron mass found in the bottom of the crucible was a small ingot called cake, typically weighing up to 2 kg . Iron prepared in this way differed from other irons by its high carbon content, up to about 1.5 %. Indeed, it is a high carbon steel. Trace elements such as vana- dium and titanium, possibly from the bamboo charcoal or other plants employed, probably contributed to the exceptional properties of this steel (§10.1).
The metallurgical know-how of India was highly appraised as early as the Pre-Islamic period . The method of preparation by fusion, ini- tially exploited in the southern part of the Indian sub-continent including Sri-Lanka, slowly propagated originally towards Asia and then towards the Middle-East, Iran, Turkey and even as far as Russia. Later, this steel will be known under the name of wootz, a name which undoubtedly comes from the English deformation of the ancient Indian word Ukko and which was stabilized at the beginning of the 19th cen- tury [16-17]. Unfortunately vestiges of this time are very rare.
According to Srinivasan and Ranganathan , one of the reasons is
perhaps that the Indians had, at least during the historic period, no funerary tradition of tombs like many other civilizations.
Thus the period during which this process was used extends from 300 BC to 1856 AD. This last date corresponds to the beginning of the modern age of iron in 1856 with the invention of the Bessemer process to manufacture molten steel on an industrial scale, which cannot be compared with the manufacturing of the Indian steel cakes. The fusion of steel was invented by Benjamin Hunstman in Sheffield in 1740, approximately two millennia after crucible steel.
Cast iron in China
Iron production by smelting appears to have been known in China from about 1000 years BC. However, China was the first country to use cast iron (i.e. molten) in around the 6th and 5th centuries BC [1, 18-21].
Among the vestiges which support this discovery are cast iron caul- drons dating from 512 BC and cast iron molds from the end of the first millennium BC. It has been suggested that these developments were made easier by the presence of phosphorus-rich ores, since phosphorus lowers the melting point of the carbon-iron alloy. Furthermore, techni- cal know-how in related fields was more advanced in China than in other parts of the world. For example, in the case of pottery, the Chi- nese mastered the manufacture of both red pottery, baked in oxidizing atmospheres, and black and egg-shell pottery baked in reducing envi- ronments. Their furnaces were ingeniously designed and made from high quality clay refractories, and bellows were in regular use in the 4th century BC. Their superiority was maintained by improvements such as the introduction of piston bellows in the 2nd century BC, and the replacement of charcoal by coal in the 3rd century BC, nearly two thousand years before Europe.
Several original techniques were developed to transform white cast iron into iron and steel by decarburizing heat treatment and also under the combined decarburizing action of forging and heating. Under the Han dynasty, in the 2nd century BC, cast iron was decarburized to transform it into ductile iron. Early in the 5th century AD, an original iron carburizing technique was developed, consisting in immersing rough iron in cast iron and then subjecting the coated product to a
phite iron, invented in... 1948! Chemical analysis revealed none of the nucleation agents used today for spheroidization. It has been suggested that an appropriate Mn/S ratio enables graphitization of cementite to occur in the solid state with a nodular morphology [22-23].
Iron making in Africa
In Equatorial Africa, neolithic practices were directly followed by an iron age, with no intermediate use of copper or bronze. The analysis and dating of many small artifacts indicates that the metallurgy of iron in this area goes back to at least the 3rd millennium BC, and possibly even to the 4th . In Gabon, furnaces dug into the soil have been carbon dated to the 7th century BC, based on charcoal residues found in the vicinity. However, the lack of spatial coincidence does not pro- vide unambiguous proof. Furthermore, iron objects remain relatively rare, due to the difficulty of conservation in the prevailing moist cli- mate and acidic soils.
It has been suggested that liquid iron was obtained at an early stage in prehistoric furnaces found near Lake Victoria in Tanzania, high tempe- ratures being attained by the injection of preheated air. However, what is probably more important is that, in the region concerned, the iron ore is extremely rich in phosphorus, while the local vegetable matter mixed with the ore is also rich in phosphorus, facilitating melting.
From Asia Minor to Europe
Around 1500 BC iron smelting was practiced in the Caucasus region Northeast of Turkey. The metallurgical know-how propagated slowly.
Towards 600 BC, the Etruscans and the Catalans practiced an advanced metallurgy. And in 300 BC, the Celtic culture spread as far as Ireland.
The metallurgical culture expanded over all of Europe. The following well documented books can be used as initiation to the history of iron specifically to this period : [18, 25-29].
The competition between bronze and iron swords lasted for several centu- ries. The Romans, who had conquered territories in Spain containing rich deposits of copper ores, used bronze swords. They did not see the advan-
, M. Collardelle et E. Verdel, “Le mobilier métallique : typologie”, Les habitats du lac de Paladru (Isère) dans leur environnement, dAF 40, Editions de la maison des sciences de l’homme, Paris (1993), 204-219.
, C. Forrières, P. Merluzzo et A. Ploquin, “La métallurgie du fer”, Les habitats du lac de Paladru (Isère) dans leur environnement, dAF 40, Editions de la maison des sciences de l’homme, Paris (1993), 220-237.
, B. Zschokke, “Du Damassé et des lames de damas”, Rev. Mét. Part I, 21, (1924), 635-669.
 C. Panseri, “L’acciaio di Damasco nelle legenda e nelle realtà”, ARMI ANTICHE, Bollettino del Accademia di S. Marciano, Torino (1962).
, J. Wadworth and O. Sherby, “On the Bulat-Damascus Steels Revisited” Progress Materials Science, 25, (1980), 35-68.
, J.D. Verhoeven, A.H. Pendray, and W.E. Dauksch, “The Key Role of Impurities in Ancient Damascus Steel Blades” JOM, Sept. 1998, 58-64.
, J.D. Verhoeven, A.H. Pendray, and E.D. Gibson, “Wootz Damascus Steel Bla- des”, Mater. Char. 37 (1996), 9-22.
, R Zeller, und Ernst Rohrer, “Orientalische Sammlung Henri Moser-Charlotten- fels. Beschreibender Katalog der Waffensammlung, Bern 1955
, L. Kapp, H. Kapp and Y. Yoshihara, The Craft of the Japanese Sword, Ed.
Kodansha Int. (1987), Tokyo, Japan.
, L. Kapp, H. Kapp and Y. Yoshihara, Modern Japanese Swords and Swordsmiths, Ed. Kodansha Int. Tokyo, (2002).
, E.C. Bain, “Nippon-tô, an introduction to old swords of Japan”, J.I.S.I. April 1962, 265-282.
, H. Tanimura, “Development of the Japanese Sword”, J. of metals, Feb 1980, 63-73.
, Tatsuo Inoue, “Japanese sword”, Materials Science Research International, 2 N°4 (1997), 193-203.
, Tatsuo Inoue, “Japanese swords in comparison with others”, in Progress in Mechanical Behaviour of Materials Proceedings ICM8 II Materials Pro- perties Ed. F. Ellyin, J.M. Provan (1999).
, Acier DAMAS. L’acier corroyé occidental. Ed. Musée de la coutellerie de Thiers, Maison des couteliers, (1999) CDrom.
, J.D. Verhoeven, and H.F Clark, “Carbon Diffusion Berween the Layers in Modern Pattern-Welded Damascus blades”, 41 (1998), 183-191.
, M. Durand-Charre, Microstructure of steels and cast irons, Ed. Springer, (2004), Berlin.
, M. Pohl, “Gefüge und Eigenschaften von Damast- und Duplexstälen”, Forts- chritte in der Metallographie, Ed. P. Portella, 2002, 254-261.
versity, Canada, Internet, (2003)
, Manouchehr M. Khorasani, “Reviving the ancient art of making persian crucible steel for bladed weaponry”, Journal of Asian Martial Arts, 17, 1, 54, (2008).
, G. Krauss, Principles of heat treatments of steels , Ed. ASM USA (1980).
 H.K.D.H. Bhadeshia, R.W.K. Honeycombe, Steels: Microstructure and Proper- ties, Butterworth-Heinemann Ltd; 3rd Revised edition edition (2006).
, J.D. Verhoeven, Steel Metallurgy for the Non-Metallurgist, ASM International, (2011).
, G. Béranger et D. Henriet, “Coloration des aciers inoxydables”, Techniques de l’Ingénieur, traité des matériaux métalliques, M 1 572, 1-11.
, Höganäs iron and steels powders for sintered components. Höganäs, (1998).
, Metallography, Höganäs Handbook for sintered components. Höganäs, (1999).
, B. Lacey and C.R. Brooks, “Microstructural Analysis of a Welded Damacus Knife Blade Billet”, Mater. Char. 29 (1992), 243-248.
, M. Durand-Charre1, F. Roussel-Dherbey et S. Coindeau, “Les aciers damassés décryptés”, Revue de Métallurgie 107, 131–143 (2010).
, J. Maréchal, “La nitruration du fer était utilisée par les anciens”, Métaux, 391 mars 1958, 133-137.
, J.D. Verhoeven, A.H. Pendray, and W.E. Dauksch, “The Continuing Study of Damacus Steel: Bars from the Alwar Armory” JOM, Sept. 2004, 17-20.
, O.D. Sherby and J. Wadsworth, “Damascus Steel” Scientific American, 252 (1985), 112-120.
, O.D. Sherby, T Oyama, D.W. Kulm, B. Walser and J. Wadsworth, “Ultrahigh Carbon Steels” JOM, june 1985, 50-56.
, O.D. Sherby and J. Wadsworth, “Comments on Damascus Steel, Part III : The Wadsworth-Sherby Mechanism by Verhoeven et al.”, Mater. Char. 28 (1992), 165-172.
, E.M. Taleff, B.L. Bramfitt, C.K. Syn, D.R. Lesuer, J. Wadsworth, and O.D.
Sherby, “Processing, structure, and properties of a rolled ultrahigh-carbon steel plate exhibiting a damask pattern”, Materials Characterization 46 (1), (2001), 11-18.